#------------------------------------------------------------------------------
#$Date: 2016-03-26 19:23:19 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180432 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/01/7210124.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7210124
loop_
_publ_author_name
'Chen, Zhaofei'
'An, Haiyan'
'Zhang, Hua'
'Hu, Ying'
_publ_section_title
;
 Metal(ii)-directed self-assembly of amino acid functionalized
 polyoxometalates
;
_journal_issue                   23
_journal_name_full               CrystEngComm
_journal_page_first              4711
_journal_paper_doi               10.1039/c3ce40129d
_journal_volume                  15
_journal_year                    2013
_chemical_formula_sum            'C12 H50 Co Mo8 N4 O40'
_chemical_formula_weight         1717.01
_chemical_name_systematic
;
?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                117.4250(10)
_cell_angle_beta                 90.1110(10)
_cell_angle_gamma                110.3570(10)
_cell_formula_units_Z            1
_cell_length_a                   9.7785(8)
_cell_length_b                   11.6587(9)
_cell_length_c                   12.0337(9)
_cell_measurement_reflns_used    5025
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.00
_cell_measurement_theta_min      2.07
_cell_volume                     1119.78(15)
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 0.01
_diffrn_measured_fraction_theta_full 0.893
_diffrn_measured_fraction_theta_max 0.893
_diffrn_measurement_device_type  'Bruker Smart Apex CCD'
_diffrn_measurement_method       ω-2θ
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0159
_diffrn_reflns_av_sigmaI/netI    0.0264
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            5025
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         2.07
_diffrn_standards_decay_%        none
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    2.640
_exptl_absorpt_correction_T_max  0.590
_exptl_absorpt_correction_T_min  0.482
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'ABSCOR by T.Higashi 8 March, 1995'
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    2.546
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             833
_exptl_crystal_size_max          0.28
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.20
_refine_diff_density_max         1.325
_refine_diff_density_min         -0.857
_refine_diff_density_rms         0.146
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.125
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     313
_refine_ls_number_reflns         3529
_refine_ls_number_restraints     18
_refine_ls_restrained_S_all      1.136
_refine_ls_R_factor_all          0.0359
_refine_ls_R_factor_gt           0.0343
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0462P)²+6.2606P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0969
_refine_ls_wR_factor_ref         0.0982
_reflns_number_gt                3360
_reflns_number_total             3529
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3ce40129d.txt
_cod_data_source_block           6
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_cell_volume        1119.77(15)
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               7210124
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Mo1 Mo 0.65590(5) 0.46800(5) 0.00988(5) 0.01703(14) Uani 1 1 d .
Mo2 Mo 0.72862(6) 0.80838(5) 0.25361(5) 0.02226(15) Uani 1 1 d .
Mo3 Mo 0.45428(6) 0.54720(5) 0.25306(5) 0.02099(15) Uani 1 1 d .
Mo4 Mo 0.10735(6) 0.24321(5) -0.00635(5) 0.02147(15) Uani 1 1 d .
Co1 Co 0.5000 1.0000 0.0000 0.0271(3) Uani 1 2 d S
O1 O 0.5276(4) 0.6210(4) 0.1106(4) 0.0193(8) Uani 1 1 d .
O2 O 0.8121(5) 0.6426(4) 0.1187(4) 0.0221(9) Uani 1 1 d .
O3 O 0.7761(5) 0.8472(4) 0.1134(4) 0.0243(9) Uani 1 1 d .
O4 O 0.6539(5) 0.6827(4) 0.3233(4) 0.0256(9) Uani 1 1 d .
O5 O 0.3088(5) 0.4235(4) 0.0966(4) 0.0224(9) Uani 1 1 d .
O6 O 0.7452(5) 0.3593(4) -0.0661(4) 0.0275(10) Uani 1 1 d .
O7 O 0.8968(6) 0.9021(5) 0.3538(5) 0.0396(12) Uani 1 1 d .
O8 O 0.6283(6) 0.9127(5) 0.3119(5) 0.0395(12) Uani 1 1 d .
O9 O 0.5858(5) 0.4204(4) 0.1237(4) 0.0234(9) Uani 1 1 d .
O10 O 0.4358(6) 0.4472(5) 0.3251(5) 0.0376(12) Uani 1 1 d .
O11 O 0.3650(5) 0.6563(5) 0.3333(5) 0.0354(11) Uani 1 1 d .
O12 O 0.0967(6) 0.1770(5) 0.0932(5) 0.0366(12) Uani 1 1 d .
O13 O -0.0635(5) 0.1537(5) -0.1052(5) 0.0384(12) Uani 1 1 d .
O14 O 0.0412(5) 0.4067(5) 0.1100(5) 0.0322(11) Uani 1 1 d .
O15 O -0.1242(6) 0.3143(5) 0.2046(6) 0.0502(15) Uani 1 1 d .
C1 C -0.0384(7) 0.4126(7) 0.1950(6) 0.0289(14) Uani 1 1 d .
C2 C -0.0099(13) 0.5626(8) 0.2987(8) 0.065(3) Uani 1 1 d .
C3 C 0.0240(17) 0.5985(14) 0.4264(12) 0.032(3) Uani 0.50 1 d P
C3A C -0.0878(18) 0.5958(18) 0.3967(16) 0.043(4) Uani 0.50 1 d P
C4 C 0.0086(11) 0.7388(9) 0.5272(8) 0.057(3) Uani 1 1 d .
C5 C -0.1293(15) 0.7272(14) 0.5827(13) 0.090(4) Uani 1 1 d U
H5A H -0.2130 0.6555 0.5136 0.108 Uiso 1 1 calc R
H5B H -0.1237 0.6927 0.6414 0.108 Uiso 1 1 calc R
C6 C -0.1625(15) 0.8454(12) 0.6468(12) 0.086(4) Uani 1 1 d U
H6A H -0.1913 0.8647 0.5821 0.103 Uiso 1 1 calc R
H6B H -0.0694 0.9226 0.6989 0.103 Uiso 1 1 calc R
N1 N 0.0590(6) 0.6631(5) 0.2529(5) 0.0273(12) Uani 1 1 d .
H1A H 0.0708 0.7491 0.3129 0.041 Uiso 1 1 calc R
H1B H 0.0005 0.6389 0.1824 0.041 Uiso 1 1 calc R
H1C H 0.1471 0.6619 0.2359 0.041 Uiso 1 1 calc R
N2 N -0.2703(8) 0.8562(8) 0.7269(7) 0.0524(18) Uani 1 1 d .
H2A H -0.2736 0.9406 0.7580 0.079 Uiso 1 1 calc R
H2B H -0.2451 0.8446 0.7910 0.079 Uiso 1 1 calc R
H2C H -0.3592 0.7901 0.6816 0.079 Uiso 1 1 calc R
O1W O 0.4240(6) 0.9199(5) 0.1274(5) 0.0422(13) Uani 1 1 d .
O2W O 0.7145(5) 1.0260(5) 0.0544(6) 0.0457(14) Uani 1 1 d .
O3W O 0.4597(6) 0.8034(5) -0.1526(5) 0.0408(12) Uani 1 1 d .
O4W O 0.3139(8) 0.9228(8) 0.4114(7) 0.080(2) Uani 1 1 d .
O5W O 0.419(2) 0.692(2) -0.4162(13) 0.127(7) Uani 0.60 1 d P
O6W O 0.443(2) 0.827(2) -0.395(2) 0.088(6) Uani 0.40 1 d PU
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O6 Mo1 O9 103.9(2) . .
O6 Mo1 O2 103.8(2) . .
O9 Mo1 O2 99.61(19) . .
O6 Mo1 O1 102.0(2) . 2_665
O9 Mo1 O1 98.28(18) . 2_665
O2 Mo1 O1 143.85(18) . 2_665
O6 Mo1 O5 99.10(19) . 2_665
O9 Mo1 O5 156.96(18) . 2_665
O2 Mo1 O5 76.40(17) . 2_665
O1 Mo1 O5 74.88(16) 2_665 2_665
O6 Mo1 O1 178.14(19) . .
O9 Mo1 O1 77.67(16) . .
O2 Mo1 O1 76.92(16) . .
O1 Mo1 O1 76.60(16) 2_665 .
O5 Mo1 O1 79.34(15) 2_665 .
O6 Mo1 Mo3 91.68(16) . 2_665
O9 Mo1 Mo3 141.12(14) . 2_665
O2 Mo1 Mo3 111.12(12) . 2_665
O1 Mo1 Mo3 43.13(12) 2_665 2_665
O5 Mo1 Mo3 34.74(11) 2_665 2_665
O1 Mo1 Mo3 86.46(10) . 2_665
O6 Mo1 Mo4 98.11(14) . 2_665
O9 Mo1 Mo4 137.87(14) . 2_665
O2 Mo1 Mo4 39.68(12) . 2_665
O1 Mo1 Mo4 111.77(12) 2_665 2_665
O5 Mo1 Mo4 37.64(11) 2_665 2_665
O1 Mo1 Mo4 81.30(9) . 2_665
Mo3 Mo1 Mo4 72.126(16) 2_665 2_665
O6 Mo1 Mo1 145.35(16) . 2_665
O9 Mo1 Mo1 86.02(14) . 2_665
O2 Mo1 Mo1 107.21(13) . 2_665
O1 Mo1 Mo1 43.32(12) 2_665 2_665
O5 Mo1 Mo1 73.89(11) 2_665 2_665
O1 Mo1 Mo1 33.28(10) . 2_665
Mo3 Mo1 Mo1 62.919(17) 2_665 2_665
Mo4 Mo1 Mo1 95.88(2) 2_665 2_665
O7 Mo2 O8 105.6(3) . .
O7 Mo2 O4 95.0(2) . .
O8 Mo2 O4 101.4(2) . .
O7 Mo2 O3 100.6(2) . .
O8 Mo2 O3 95.7(2) . .
O4 Mo2 O3 152.88(18) . .
O7 Mo2 O1 159.8(2) . .
O8 Mo2 O1 92.6(2) . .
O4 Mo2 O1 72.52(16) . .
O3 Mo2 O1 85.87(16) . .
O7 Mo2 O2 90.6(2) . .
O8 Mo2 O2 162.2(2) . .
O4 Mo2 O2 84.24(16) . .
O3 Mo2 O2 73.59(16) . .
O1 Mo2 O2 72.73(14) . .
O7 Mo2 Mo3 126.16(17) . .
O8 Mo2 Mo3 89.89(17) . .
O4 Mo2 Mo3 31.21(13) . .
O3 Mo2 Mo3 129.37(13) . .
O1 Mo2 Mo3 43.55(10) . .
O2 Mo2 Mo3 86.36(10) . .
O7 Mo2 Mo4 90.35(18) . 2_665
O8 Mo2 Mo4 127.04(18) . 2_665
O4 Mo2 Mo4 127.65(13) . 2_665
O3 Mo2 Mo4 31.35(12) . 2_665
O1 Mo2 Mo4 85.30(10) . 2_665
O2 Mo2 Mo4 43.59(10) . 2_665
Mo3 Mo2 Mo4 120.647(19) . 2_665
O10 Mo3 O11 104.8(2) . .
O10 Mo3 O4 103.3(2) . .
O11 Mo3 O4 98.1(2) . .
O10 Mo3 O5 103.9(2) . .
O11 Mo3 O5 98.3(2) . .
O4 Mo3 O5 143.27(18) . .
O10 Mo3 O1 156.0(2) . .
O11 Mo3 O1 99.2(2) . .
O4 Mo3 O1 73.18(16) . .
O5 Mo3 O1 71.87(16) . .
O10 Mo3 O9 85.4(2) . .
O11 Mo3 O9 169.8(2) . .
O4 Mo3 O9 78.80(17) . .
O5 Mo3 O9 79.35(16) . .
O1 Mo3 O9 70.61(14) . .
O10 Mo3 Mo1 142.66(18) . 2_665
O11 Mo3 Mo1 89.88(17) . 2_665
O4 Mo3 Mo1 108.44(13) . 2_665
O5 Mo3 Mo1 39.16(12) . 2_665
O1 Mo3 Mo1 35.56(10) . 2_665
O9 Mo3 Mo1 82.04(10) . 2_665
O10 Mo3 Mo2 134.95(18) . .
O11 Mo3 Mo2 90.88(16) . .
O4 Mo3 Mo2 31.85(13) . .
O5 Mo3 Mo2 115.43(12) . .
O1 Mo3 Mo2 43.61(10) . .
O9 Mo3 Mo2 81.38(10) . .
Mo1 Mo3 Mo2 77.475(17) 2_665 .
O12 Mo4 O13 105.6(2) . .
O12 Mo4 O3 98.2(2) . 2_665
O13 Mo4 O3 101.8(2) . 2_665
O12 Mo4 O14 96.2(2) . .
O13 Mo4 O14 89.7(2) . .
O3 Mo4 O14 158.39(17) 2_665 .
O12 Mo4 O5 97.4(2) . .
O13 Mo4 O5 153.5(2) . .
O3 Mo4 O5 87.56(17) 2_665 .
O14 Mo4 O5 74.65(17) . .
O12 Mo4 O2 164.6(2) . 2_665
O13 Mo4 O2 89.4(2) . 2_665
O3 Mo4 O2 74.87(16) 2_665 2_665
O14 Mo4 O2 87.14(16) . 2_665
O5 Mo4 O2 68.95(15) . 2_665
O12 Mo4 Mo2 130.34(17) . 2_665
O13 Mo4 Mo2 90.45(17) . 2_665
O3 Mo4 Mo2 32.16(13) 2_665 2_665
O14 Mo4 Mo2 131.22(13) . 2_665
O5 Mo4 Mo2 84.44(11) . 2_665
O2 Mo4 Mo2 44.09(10) 2_665 2_665
O12 Mo4 Mo1 135.02(17) . 2_665
O13 Mo4 Mo1 117.89(18) . 2_665
O3 Mo4 Mo1 84.32(12) 2_665 2_665
O14 Mo4 Mo1 74.10(12) . 2_665
O5 Mo4 Mo1 37.68(11) . 2_665
O2 Mo4 Mo1 32.07(10) 2_665 2_665
Mo2 Mo4 Mo1 63.055(15) 2_665 2_665
O3W Co1 O3W 180.0(2) 2_675 .
O3W Co1 O2W 89.3(2) 2_675 .
O3W Co1 O2W 90.7(2) . .
O3W Co1 O2W 90.7(2) 2_675 2_675
O3W Co1 O2W 89.3(2) . 2_675
O2W Co1 O2W 180.0 . 2_675
O3W Co1 O1W 86.42(19) 2_675 .
O3W Co1 O1W 93.58(19) . .
O2W Co1 O1W 90.2(2) . .
O2W Co1 O1W 89.8(2) 2_675 .
O3W Co1 O1W 93.58(19) 2_675 2_675
O3W Co1 O1W 86.42(19) . 2_675
O2W Co1 O1W 89.8(2) . 2_675
O2W Co1 O1W 90.2(2) 2_675 2_675
O1W Co1 O1W 180.0(2) . 2_675
Mo1 O1 Mo3 101.31(16) 2_665 .
Mo1 O1 Mo2 154.0(2) 2_665 .
Mo3 O1 Mo2 92.84(15) . .
Mo1 O1 Mo1 103.40(16) 2_665 .
Mo3 O1 Mo1 96.23(15) . .
Mo2 O1 Mo1 96.48(15) . .
Mo1 O2 Mo4 108.26(19) . 2_665
Mo1 O2 Mo2 112.76(19) . .
Mo4 O2 Mo2 92.33(15) 2_665 .
Mo4 O3 Mo2 116.5(2) 2_665 .
Mo3 O4 Mo2 116.9(2) . .
Mo3 O5 Mo4 148.0(2) . .
Mo3 O5 Mo1 106.10(18) . 2_665
Mo4 O5 Mo1 104.69(18) . 2_665
Mo1 O9 Mo3 115.5(2) . .
C1 O14 Mo4 128.2(4) . .
O15 C1 O14 127.2(6) . .
O15 C1 C2 119.0(6) . .
O14 C1 C2 113.7(6) . .
C3A C2 C3 48.2(9) . .
C3A C2 N1 120.3(9) . .
C3 C2 N1 121.9(9) . .
C3A C2 C1 124.3(10) . .
C3 C2 C1 118.5(9) . .
N1 C2 C1 110.6(6) . .
C3A C3 C2 65.1(11) . .
C3A C3 C4 70.9(12) . .
C2 C3 C4 115.1(11) . .
C3 C3A C2 66.7(11) . .
C3 C3A C4 67.7(12) . .
C2 C3A C4 114.0(12) . .
C5 C4 C3 118.4(9) . .
C5 C4 C3A 89.2(9) . .
C3 C4 C3A 41.4(7) . .
C6 C5 C4 119.5(11) . .
C6 C5 H5A 107.4 . .
C4 C5 H5A 107.4 . .
C6 C5 H5B 107.4 . .
C4 C5 H5B 107.4 . .
H5A C5 H5B 107.0 . .
C5 C6 N2 124.5(10) . .
C5 C6 H6A 106.2 . .
N2 C6 H6A 106.2 . .
C5 C6 H6B 106.2 . .
N2 C6 H6B 106.2 . .
H6A C6 H6B 106.4 . .
C2 N1 H1A 109.5 . .
C2 N1 H1B 109.5 . .
H1A N1 H1B 109.5 . .
C2 N1 H1C 109.5 . .
H1A N1 H1C 109.5 . .
H1B N1 H1C 109.5 . .
C6 N2 H2A 109.5 . .
C6 N2 H2B 109.5 . .
H2A N2 H2B 109.5 . .
C6 N2 H2C 109.5 . .
H2A N2 H2C 109.5 . .
H2B N2 H2C 109.5 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O6 1.706(4) .
Mo1 O9 1.759(4) .
Mo1 O2 1.888(4) .
Mo1 O1 1.925(4) 2_665
Mo1 O5 2.134(4) 2_665
Mo1 O1 2.408(4) .
Mo1 Mo3 3.2467(8) 2_665
Mo1 Mo4 3.3774(7) 2_665
Mo1 Mo1 3.4136(10) 2_665
Mo2 O7 1.697(5) .
Mo2 O8 1.727(5) .
Mo2 O4 1.942(4) .
Mo2 O3 1.957(4) .
Mo2 O1 2.266(4) .
Mo2 O2 2.291(4) .
Mo2 Mo3 3.2813(7) .
Mo2 Mo4 3.2908(7) 2_665
Mo3 O10 1.711(5) .
Mo3 O11 1.719(5) .
Mo3 O4 1.907(4) .
Mo3 O5 1.926(4) .
Mo3 O1 2.264(4) .
Mo3 O9 2.339(4) .
Mo3 Mo1 3.2467(8) 2_665
Mo4 O12 1.684(5) .
Mo4 O13 1.712(5) .
Mo4 O3 1.913(4) 2_665
Mo4 O14 2.101(4) .
Mo4 O5 2.132(4) .
Mo4 O2 2.271(4) 2_665
Mo4 Mo2 3.2908(7) 2_665
Mo4 Mo1 3.3774(7) 2_665
Co1 O3W 2.067(5) 2_675
Co1 O3W 2.067(5) .
Co1 O2W 2.071(5) .
Co1 O2W 2.071(5) 2_675
Co1 O1W 2.148(5) .
Co1 O1W 2.148(5) 2_675
O1 Mo1 1.925(4) 2_665
O2 Mo4 2.271(4) 2_665
O3 Mo4 1.913(4) 2_665
O5 Mo1 2.134(4) 2_665
O14 C1 1.278(8) .
O15 C1 1.218(8) .
C1 C2 1.530(9) .
C2 C3A 1.382(16) .
C2 C3 1.398(15) .
C2 N1 1.476(9) .
C3 C3A 1.13(2) .
C3 C4 1.586(15) .
C3A C4 1.62(2) .
C4 C5 1.497(14) .
C5 C6 1.389(15) .
C5 H5A 0.9700 .
C5 H5B 0.9700 .
C6 N2 1.429(11) .
C6 H6A 0.9700 .
C6 H6B 0.9700 .
N1 H1A 0.8900 .
N1 H1B 0.8900 .
N1 H1C 0.8900 .
N2 H2A 0.8900 .
N2 H2B 0.8900 .
N2 H2C 0.8900 .
O5W O6W 1.41(3) .
